### SlideShare for iOS

by Linkedin Corporation

FREE - On the App Store

- Total Views
- 3,601
- Views on SlideShare
- 3,601
- Embed Views

- Likes
- 4
- Downloads
- 178
- Comments
- 0

No embeds

Uploaded via SlideShare as Adobe PDF

© All Rights Reserved

- 1. Diffraction BasicsIntroductionThe utilization of X-ray diffraction for crystallographic analysis relies on a few basicprincipals: 1. When an incident beam of x-rays interacts with a target material, one of the primary effects observed is scattering (spherical radiation of the incident x-rays without change in wavelength) of those x-rays from atomic scattering centers within the target material. 2. In materials with some type of regular (i.e., crystalline) structure, x-rays scattered in certain directions will be in-phase (i.e., amplified), while most will be out of phase. This is the process of diffraction. 3. Measurement of the geometry of the diffracted x-rays can be used to discern the crystal structure and unit cell dimensions of the target material. 4. The intensities of the amplified x-rays can be used to work out the arrangement of atoms in the unit cell.For the x-rays to yield useful information about the material structure, the wavelength of theincident x-rays should be of that same order of magnitude as the interatomic spacing in thecrystal structure.In this section we will discuss this process of diffraction and how we make use of theamplification and attenuation to elucidate the structure of the material(s) in the target. Thegoal of this section is to give the student sufficient background in the mathematics andcrystallography underlying the practice of x-ray diffraction so that the analytical results willrise above the level of a “black box” technique.The first part of the material (including the illustrations) in this section is abstracted fromChapter 3 of Nuffield (1966). The remainder of the material (from Bragg’s Law on and thereciprocal lattice) is from Jenkins and Snyder (1996) and Bloss (1994). I thank Dr. CornelisKlein for his suggestions and assistance with this material.The Geometry of DiffractionAs discussed previously, there are many typesof secondary effects that occur when x-raysinteract with matter. Fortunately the dominanteffect, and the only one with which we areconcerned in diffraction, is scattering. In thisprocess, an electron in the path of the x-raybeam vibrates with the frequency of theincoming radiation thus becomes a secondarypoint source of x-rays of the same energy as theincident x-rays (Fig 3-1). The atom (or itsnucleus) is not actually the point source of x-rays, but the electrons surrounding the atom willscatter x-rays that appear to emanate from the(Revision date: 19-Feb-03) Page 1 of 18
- 2. Diffraction Basicscenter of the atom.A crystal is a complex but orderly arrangement of atoms, and all atoms in the path of an x-ray beam scatter x-rays simultaneously. In general, the scattered x-rays interfere, essentiallycanceling each other out. In certain specific directions, where the scattered x-rays are “in-phase” the x-rays scatter cooperatively to form a new wave. This process of constructiveinterference is diffraction.The directions of possible diffractions depend only on the size and shape of the unit cell.Certain classes of diffraction are systematically extinguished by lattice centering and bycertain space-group symmetry elements. The intensities of the diffracted waves depend onthe kind and arrangement of atoms in the crystal structure. It is the study of the geometry ofdiffraction from a crystal that we use to discern the unit cell dimensions; the missingdiffractions give the symmetry of the crystal. The intensities are used to work out thearrangement of atoms.The Laue treatment of the geometry of diffraction, developed by Max von Laue in 1912, ispresented in the following sections because of its geometric clarity and the rigor with whichthe concepts are treated. As will be discussed, Laue diffraction occurs with polychromatic(i.e., “white”) rather than monochromatic radiation that we use with powder diffractometry.Later we will present Bragg’s treatment of diffraction that allow diffraction ofmonochromatic x-rays to be treated as reflection. Bragg’s treatment greatly simplifies themathematics involved in diffraction calculations, and, when combined with the somewhatdifficult but very useful concept of the reciprocal lattice, simplifies the experimentalmeasurement of a diffraction pattern, thus making diffraction a useful routine tool forcrystallographic studies.Diffraction by a Row of Identical, Equally Spaced Atoms Consider the hypothetical case of a one-dimensional row of equally spaced atoms. Each atom in the path of an x-ray beam can be considered to be the center of radiating, spherical wave shells of x-rays (Fig 3-2). In general the scattered waves interfere, cancel out and no diffraction occurs. However, when the scattered waves happen to be in phase, they form wave fronts asshown in Figure 3-2. Since wavelengths of λ, 2λ and 3λ will all add to produce a differentwavefront, we call these first-, second- and third-order wavefronts. By convention,(Revision date: 19-Feb-03) Page 2 of 18
- 3. Diffraction Basicswavefronts to the right of the diffracted beam is are positive, those to the left are negative(i.e., minus first-order, etc.). Figure 3-3. Condition for diffraction from a rowFigure 3-3 illustrates the conditions for diffraction from a row of atoms. Two x-rays strikethe row of periodicity p, at an angle of incidence µ , to form zero-, first- and second-orderdiffractions. The angle of diffraction, ν , is measured from the left (positive) end of the row.The diffracted rays are only in phase if: p (cosν − cos µ ) = ± hλwhere h is the order of the diffraction, in this case 0 or 1. The condition for diffraction is metnot only in the directions AD, AE and AF shown in the diagrams, but in all directions thatmake angles of ν , ν ′ and ν ′′ . These outline three concentric cones as shown in figure 3-3d.The cones define the locus of in-phase scattering (diffraction).(Revision date: 19-Feb-03) Page 3 of 18
- 4. Diffraction BasicsThe expression above is the Laue equation for diffraction by a row. Note that for zero-orderdiffractions, h = 0, and thatν is equal to µ . The significance of this is that the incident beamis always a line in the zero-order cone.When the angle of incidence, µ , is 90°, the Laue equation reduces to: p cosν = ± hλ Under this condition the angleν for zero order diffractions is also 90° and the zero-order cone has the shape of a disk. Higher- order cones occur in pairs, symmetrically placed about the zero-order disk (Fig. 3-4)Diffraction by a Plane Lattice-Array of AtomsA plane lattice-array of atoms (Fig. 3-5) may be defined by two translation periods, a and b,in the rows OA and OB and the angle γ. Basically this extends the concept of diffraction by arow to include simultaneous diffraction by two non-parallel rows of atoms.The diffraction directions for the row OA comprise a set of concentric cones coaxial with OA(Fig 3-5b), and have half-apical angles defined by the Laue equation for a row. Thedirections for the row OB comprise another set of cones (Fig 3-5c) with a differentorientation.When both diffractions are combined, only at the intersection of the diffraction cones willdiffraction occur (since the other diffractions will interfere and thus cancel). Those lines ofintersection are shown as OX and OY (Fig 3-5d). The Laue equations for diffraction by theplane may be expresses in terms of the Laue equations for the rows OA and OB: a(cosν 1 − cos µ1 ) = ± hλ b(cosν 2 − cos µ 2 ) = ± kλwhere a and b are periods of the rows µ1 and µ 2 are the angles at which the beam meets the rows ν 1 and ν 2 are the diffractions angles referred to the respective rows.(Revision date: 19-Feb-03) Page 4 of 18
- 5. Diffraction BasicsDiffraction occurs when the two equations are simultaneously satisfied, i.e., when the anglesν 1 and ν 2 define the same direction. As illustrated in Fig 3-5d, when the beam meets theplane at such an angle that the hth-order cone about OA intersects the kth-order cone aboutOB along OX and OY. The angle between OA and OX (and OY) is ν 1 and that between OBand OX is ν 2 .Diffraction by a Three-Dimensional Lattice-Array of Atoms The diffraction directions for a three- dimensional array may be described by three sets of diffraction cones coaxial with three non-coplanar reference rows (Fig 3- 6). In general, each cone will form two diffraction lines by intersection with each of the other two(Revision date: 19-Feb-03) Page 5 of 18
- 6. Diffraction Basicsresulting in 6 diffraction lines shown as OU and OV (a-c) , OY and OZ (a-b), OW and OX (b-c). For the material to diffract (i.e., interfere constructively) the three diffractions OV, OW,and OY would need to be coincident, a condition satisfied by the following Laue equationsonly when the diffraction angles, ν 1 , ν 2 and ν 3 define a common direction: a(cosν 1 − cos µ1 ) = ± hλ b(cosν 2 − cos µ 2 ) = ± kλ c(cosν 3 − cos µ 3 ) = ±lλThe a, b and c directions are fixed (and define the unit cell), thus the ν values depend on µ(the angle at which the beam meets the reference rows) and λ, (the wavelength of theincident radiation). The possibility of satisfying the three equations simultaneously can beincreased by varying either µ or λ during analysis. In Laue diffraction, the crystal positionin the beam is fixed, and λ is varied by using continuous (or “white”) radiation while keepingthe orientation of the crystal fixed. Monochromatic radiation is used in most moderndiffraction equipment, so for single crystal analysis the crystal must be progressively movedin the X-ray beam to vary µ sufficiently so that diffractions may be obtained and recorded.Below is a sample Laue diffraction pattern (Fig 7.39 from Klein, 2002).The table below summarizes the different diffraction methods and the radiation used. Mostof this course will be concerned with powder methods.(Revision date: 19-Feb-03) Page 6 of 18
- 7. Diffraction Basics Radiation Method White Laue: stationary single crystal Monochromatic Powder: specimen is polycrystalline, and therefore all orientations are simultaneously presented to the beam Rotation, Weissenberg: oscillation, De Jong-Bouman: single crystal rotates or oscillates about chosen axis in path of beam Precession: chosen axis of single crystal precesses about beam directionDiffraction as Reflection: The Bragg LawIn 1912, shortly after von Laue’s experiments were published, Sir W.L. Bragg discoveredthat diffraction could be pictured as a reflection of the incident beam from lattice planes. Hedeveloped an equation for diffraction, equivalent to the simultaneous solution of the threeLaue equations by monochromatic radiation, which allows diffraction to be treatedmathematically as reflection from the diffracting planes. Nuffield’s (1966) explanation of the Bragg condition is particularly clear. In Figure 3-7 at left, an x-ray beam encounters a three dimensional lattice- array of atoms shown as rows OA, OB and OC. In this case we assume that the third-order cone about OA, the second- order cone about OB and the first-order cone about OC intersect in a common line to satisfy the Laue condition for diffraction.1 The x-rays scattered by adjacent atoms on OA have a path difference of three wavelengths, those around OB have a path difference of two wavelengths and those around OC, one wavelength difference. These three points of coherentscatter define a plane with intercepts 2a, 3b, 6c. The Miller index of this plane (thereciprocal of the intercepts) is (321). Because A’’, B’’ and C’’ are six wavelengths out of1 Keep in mind that diffraction is not really reflection, but coherent scattering from lattice points, such that eachpoint may be thought of as an independent source of x-rays. Diffraction occurs when the scattered x-rays are inphase.(Revision date: 19-Feb-03) Page 7 of 18
- 8. Diffraction Basicsphase with those scattered at the origin, they scatter waves that differ by zero wavelengthsfrom one another. To maintain the same path length (and remain in phase) the rays must pass through the plane (Fig 3-8a) or be deviated at an angle equal to the angle of incidence, θ (Fig 3-8b). Though it is not really reflecting the X-rays, the effective geometry is that ofreflection. Since the lattice is three-dimensional and any lattice point will act as the origin,(321) defines an infinite number of parallel planes that diffract simultaneously. Therelationship may be stated as follows: A diffraction direction defined by the intersection ofthe hth order cone about the a axis, the kth order cone about the b axis and the lth ordercone about the c axis is geometrically equivalent to a reflection of the incident beam fromthe (hkl) plane referred to these axes. This geometric relation provides the basis for Braggdiffraction. Referring to Figure 3-7, diffraction from each parallel plane shown will beexactly one wavelength out of phase at the proper value of θ. Figure 3-9 shows a beam of parallel x-rays penetrating a stack of planes of spacing d, at a glancing angle of incidence, θ. Each plane is pictured as reflecting a portion of the incident beam. The “reflected” rays combine to form a diffracted beam if they differ in phase by a whole number of wavelength, that is, if the path difference AB- AD = nλ where n is an integer. Therefore d AB = and sin θ d AD = AB cos 2θ = (cos 2θ ) sin θ d dTherefore: nλ = − (cos 2θ ) sin θ sin θ d d = (1 − cos 2θ ) = (2 sin 2 θ ) sin θ sin θ nλ = 2d sin θThe last equation is the Bragg condition for diffraction.(Revision date: 19-Feb-03) Page 8 of 18
- 9. Diffraction BasicsThe value of n gives the “order” of the diffraction. Note that the value of the diffractionangle, θ, will increase as the order of diffraction increases up to the limit where nλ = 2d. Thediagram below (from Bloss, 1994) illustrates this graphically. A indicates light reflectionfrom a polished (111) face of an NaCl crystal. B indicates diffraction by Cu Kα x-rays atsuccessive orders of diffraction, with the first-order diffraction at θ = 13.7° (2θ = 25.4°). Cshows the wavelength difference producing the different orders of diffraction. Thesereflections are commonly referred to as multiples of the Miller index for the planes withoutthe parentheses, i.e., 111, 222, 333, 444, but are represent the same value of d.It can be easily shown that Bragg diffraction occurs in any set of planes in a crystal structure.Because of geometrical considerations related to multiple out-of phase diffractions (a.k.a.extinction) in some types of point groups and space groups, not all lattice planes will producemeasurable diffractions. As will be discussed later, these missing diffractions providevaluable information about the crystal structure.The Reciprocal LatticeThe most useful method for describing diffraction phenomena has the intimidating name“reciprocal lattice.” It was developed by P.P. Ewald, and is also called “reciprocal space.” Itmakes use of the reciprocal of dhkl to fabricate a geometrical construction which then servesas a very effective way to understand diffraction effects. Most of the discussion in thissection is abstracted from Jenkins and Snyder (1996).When setting up an arrangement of x-ray source, specimen and detector, it is useful to beable to predict the motions that will have to be applied the various motions that will have tobe applied to see particular diffraction effects. Consider the diffraction from the (200) planesof a (cubic) LiF crystal that has an identifiable (100) cleavage face. To use the Braggequation to determine the orientation required for diffraction, one must determine the valueof d200. Using a reference source (like the ICDD database or other tables of x-ray data) forLiF, a = 4.0270 Å, thus d200 will be ½ of a or 2.0135 Å. From Bragg’s law, the diffractionangle for Cu Kα1 (λ = 1.54060) will be 44.986° 2θ. Thus the (100) face should be placed tomake an angle of 11.03° with the incident x-ray beam and detector. If we had no more(Revision date: 19-Feb-03) Page 9 of 18
- 10. Diffraction Basicscomplicated orientation problems, then we would have no need for the reciprocal spaceconcept. Try doing this for the (246) planes and the complications become immediately evident. The orientation problem is related to the fact that the diffracting Bragg planes are inherently three dimensional. We can remove a dimension from the problem by representing each plane as a vector – dhkl is defined as the perpendicular distance from theorigin of a unit cell to the first plane In the family hkl as illustrated in Figure 3.2. While thisremoves a dimensional element, it is evident that the sheaf of vectors representing all thelattice planes (see Fig. 3.3 on the following page) will be extremely dense near the center andnot ultimately very useful.Ewald proposed that instead of plotting the dhkl vectors, that the reciprocal of these vectorsshould be plotted. The reciprocal vector is defined as: 1 d* ≡ hkl d hklFigure 3.3 can now be reconstructed plotting the reciprocal vectors instead of the dhkl vectors.Figure 3.4 shows this construction. The units are in reciprocal angstroms and the space istherefore a reciprocal space. Note that the points in this space repeat at perfectly periodicintervals defining a space lattice called a reciprocal lattice. The repeating translation vectorsin this lattice are called a*, b* and c*. The interaxial (or reciprocal) angles are α*, β* and γ*where the reciprocal of an angle is defined as its complement, or 180° minus the real-spaceangle. For orthogonal systems the angular relations are quite simple. For non-orthogonalsystems (monoclinic and triclinic), they are more complex.(Revision date: 19-Feb-03) Page 10 of 18
- 11. Diffraction Basics The reciprocal lattice makes the visualization of Bragg planes very easy. Figure 3.4 shows only the (hk0) plane of the reciprocal lattice. To establish the index of any point in the reciprocal lattice, count the number of repeat units in the a*, b*, and c* directions. Fig. 3.4 shows only the hk0 plane, but the lattice is fully three dimensional. When connected, the innermost points in the lattice will define a three-dimensionalshape that is directly related to the shape of the of the real-space unit cell. Thus the(Revision date: 19-Feb-03) Page 11 of 18
- 12. Diffraction Basicssymmetry of the real space lattice propagates into the reciprocal lattice. Any vector in thelattice represents a set of Bragg planes and can be resolved into its components: d hkl = ha * + kb * + lc * *In orthogonal crystal systems, the relationship between d and d* is a simple reciprocal. Innon-orthogonal systems (triclinic, monoclinic, hexagonal), the vector character of thereciprocals complicates the angular calculations. The figure at left shows the relations for the ac plane of a monoclinic unit cell. d001 meets the (100) plane at 90°. Because the angle β between the a and c directions is not 90°, the a unit cell direction and the d100 are not equal in magnitude or direction, but are related by the sin of the angle between them. This means that the reciprocal lattice parameters d*100 and a*will also involve the sin of the interaxial angle.Table 3.1 (at right)lists the direct andreciprocal spacerelationships in thedifferent crystalsystems. Theparameter V shownfor the Triclinicsystem is acomplicatedtrigonometriccalculation requiredfor the this systembecause of theabsence of 90°angles. It is derived by Jenkins and Snyder (1994, p. 53) and listed below: 1 V* = = a * b * c * (1 − cos 2 α * − cos 2 β * − cos 2 γ * +2 cos α * cos β * cos γ *)1 / 2 VThe Ewald Sphere of ReflectionFigure 3.6 (following page) shows a cross section through an imaginary sphere with a radiusof 1/λ with a crystal at its center. The reciprocal lattice associated with the crystal’s lattice isviewed as tangent to the sphere at the point where an x-ray beam entering from the left andpassing through the crystal would exit the sphere on the right. The Ewald sphere contains allthat is needed to visualize diffraction geometrically.(Revision date: 19-Feb-03) Page 12 of 18
- 13. Diffraction Basics Rotation of the crystal (and its associated real- space lattice) will will also rotate the reciprocal lattice because the reciprocal lattice is defined in terms of the real-space lattice. Figure 3.7 shows this arrangement at a specific time when the (230) point is broght into contact with the sphere. Here, by definition: 1 CO = and λ d *( 230 ) OA = hence 2 OA d *( 230) / 2 sin θ = = CO 1/ λ or 2 sin θ λ= d *( 230 ) from the definition of the reciprocal vector: 1 d ( 230 ) ≡ d *( 230) therefore: λ = 2d ( 230 ) sin θ which is the Bragg equation. As each latticepoint, representing a d*-value, touches the sphere of reflection, the diffraction condition ismet and diffraction occurs. In terms of Bragg notation, the real-space lattice plane,represented by d*, “reflects” the incident beam. Note that the angle between the incident x-(Revision date: 19-Feb-03) Page 13 of 18
- 14. Diffraction Basicsray beam and the diffraction point on the Ewald sphere is 2θ; this is directly related to the useof 2θ as a measurement convention in x-ray diffraction data.In the notation of the Ewald sphere, the diffracted intensity is directed from the crystal in thedirection of the lattice point touching the sphere. The Ewald sphere construction is veryuseful in explaining diffraction in a manner that avoids the need to do complicatedcalculations. It allows us to visualize and effect using a pictorial, mental model, and permitssimple analysis of otherwise complex relationships among the crystallographic axes andplanes.The Powder Diffraction PatternMethods of single crystal diffraction are not germane to this course. Most of the previousdiscussions have been in relation to diffraction by single crystals, and most modern methodsof single crystal diffractometry utilize automated three-axis diffractometers to move thespecimen in a systematic manner and obtain a diffraction pattern.Most materials are not single crystals, but are composed of billions of tiny crystallites – herecalled a polycrystalline aggregate or powder. Many manufactured and natural materials(including many rocks) are polycrystalline aggregates. In these materials there will be agreat number of crystallites in all possible orientations. When a powder with randomlyoriented crystallites is placed in an x-ray beam, the beam will see all possible interatomicplanes. If we systematically change the experimental angle we produce and detect allpossible diffraction peaks from the powder. Here’s how it works in the context of the Ewaldsphere: • There is a d*hkl vector associated with each point in the reciprocal lattice with its origin on the Ewald sphere at the point where the direct X-ray beam exists • Each crystallite located in the center of the Ewald sphere has its own reciprocal lattice with its orientation determined by the orientation of the crystallite with respect to the X-ray beam.(Revision date: 19-Feb-03) Page 14 of 18
- 15. Diffraction BasicsThe Powder CameraFigure 3.9 shows this geometry from the d*100 reflection, which forms a sphere of vectors emanating from the point of interaction with the beam. The number of vectors will be equal to the number of crystallites interacting with the x-ray beam. The angle between the beam and the cone of diffraction (refer to Fig 3.7) is 2θ. In the diagram at left (Fig 3.10), the diffraction cones from the (100) reflection are shown. In the powder camera, these rings intersect a 360° ring of film, and parts of the cones are captured on film as Debye rings, producing a Debye-Scherrer diffraction photograph. Debye-Scherrer powder cameras (illustrated at left) have been largely supplanted in analytical laboratories by automated diffractometers. The powder patterns recorded on film in these devices accurately record the true shape of the diffraction cones produced.(Revision date: 19-Feb-03) Page 15 of 18
- 16. Diffraction Basics The schematic at left shows the Debye cones that intersect the film in the camera, and how diffractions are measured on the film to determine the d-spacings for the reflections measured. Two Debye- Scherrer powder camera photographs are shown below. The upper film is gold (Au), a Face centered cubic structure (Fm3m) that exhibits a fairly simple diffractionpattern.The film below is of Zircon (ZrSiO4). Zircon is a fairly complex tetragonal structure(4/m2/m2/m) and this complexity is reflected in the diffraction pattern.The Powder DiffractometerMost modern X-ray diffraction laboratories rely on automated powder diffractometers.While diffractometers differ in the geometry, their purpose is the measurement of the dhklvalues and diffraction intensities for powder specimens. In essence, the powderdiffractometer is designed to measure diffractions occurring along the Ewald sphere from apowder specimen. It can be thought of as a system for moving through the reciprocal lattice,measuring d-spacings as they occur. By convention (but not by accident – see Fig. 3.7)diffraction angles are recorded at 2θ. We will discuss our Scintag diffractometer in moredetail later in this course.Figure 7.4 (following page from Jenkins and Snyder, 1996) shows the geometry and commonmechanical movements in the different types of diffractometers. The table shows the(Revision date: 19-Feb-03) Page 16 of 18
- 17. Diffraction Basicsdiffractometer type, and how the various components move (or don’t move). In the table r1 isthe distance between the tube (usually taken as the anode) and the specimen, and r2 thedistance between the specimen and the receiving slit.The Seeman-Bolin diffractometer fixes the incident beam and specimen and moves thereceiving slit (detector) assembly, varying r2 with 2θ to maintain the correct geometry.The Bragg-Brentano diffractometer is the dominant geometry found in most laboratories. Inthis system, if the tube is fixed, this is called θ-2θ geometry. If the tube moves (and thespecimen is fixed), this is called θ:θ geometry. The essential characteristics are: • The relationship between θ (the angle between the specimen surface and the incident x-ray beam) and 2θ (the angle between the incident beam and the receiving slit- detector) is maintained throughout the analysis. • r1 and r2 are fixed and equal and define a diffractometer circle in which the specimen is always at the center.A detailed schematic of this geometry is on the following page (Fig. 7.6 from Jenkins andSnyder).(Revision date: 19-Feb-03) Page 17 of 18
- 18. Diffraction BasicsThe arrangement above includes the following elements: • F – the X-ray source • DS – the divergence scatter slit • SS –Soller slit assembly (SS1 on “tube” side, SS2 on detector side), a series of closely spaced parallel plates, parallel to the diffractometer circle (i.e., the plane of the paper), designed to limit the axial divergence of the beam. • α -- the “take off” angle – the angle between the anode surface and the primary beam • θ and 2θ are as defined above. • RS – the receiving slit, located on the diffractometer circle (which remains fixed throughout diffractometer movement) • C – the monochromator crystal. rm is the radius of the monochromator circle on which RS, C and AS (the detector slit) lie. • rf is the radius of the focusing circle. F, S and RS all fall on this circle. rf is very large at low θ values and decreases as θ increases.We will discuss the Bragg-Brentano diffractometer in more detail in subsequent weeks.ConclusionsThis introduction to diffraction has been primarily concerned with development of anunderstanding of the source of diffraction and understanding how crystalline spacings can bedetermined experimentally by x-ray diffraction methods.What is missing in the treatment so far is related to the intensity of diffraction. Basically notall diffractions are created equal – some are much more intense than others and some that oneassumes should be present are missing altogether. The source of the variations in intensity ofdiffraction and the relationship to crystal structure and chemistry will be the topic of Part 2.(Revision date: 19-Feb-03) Page 18 of 18

Full NameComment goes here.bala subrahmanyam, physics lecturer at bapatla engineering college 2 months agoAlaa Hassan7 months agoreyhane mazahernasab, student at international university of imam khomeini 1 year agoHarendra Bhardwaj1 year ago